Synthesis, Structures, and Magnetic Properties of Rare-Earth Cobalt Arsenides, RCo2As2(R = La, Ce, Pr, Nd)
Thompson, Corey M.; Tan, Xiaoyan; Kovnir, Kirill; Garlea, V. Ovidiu; Gippius, Andrei A.; Yaroslavtsev, Alexander A.; Menushenkov, Alexey P.; Chernikov, Roman V.; Büttgen, Norbert; Krätschmer, Wolfgang; Zubavichus, Yan V.; Shatruk, Michael; Chemistry of Materials 26 (2014) 3825–; doi:10.1021/cm501522v

data_4001991
_publ_section_title
;
 Synthesis, Structures, and Magnetic Properties of Rare-Earth Cobalt
 Arsenides, RCo2As2(R = La, Ce, Pr, Nd)
;
_journal_issue                   12
_journal_name_full               'Chemistry of Materials'
_journal_page_first              3825
_journal_paper_doi               10.1021/cm501522v
_journal_volume                  26
_journal_year                    2014
_chemical_formula_sum            'As2 Bi0.05 Ce0.95 Co1.83'
_chemical_formula_weight         401.54
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           139
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           manual
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   4.03090(10)
_cell_length_b                   4.03090(10)
_cell_length_c                   10.2591(4)
_cell_measurement_temperature    293(2)
_cell_volume                     166.691(9)
_computing_cell_refinement       'SMART V5.625 (Bruker, 2000)'
_computing_data_collection       'SMART V5.625 (Bruker, 2000)'
_computing_data_reduction        'SAINT V6.32 (Bruker, 2001)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  'Bruker APEX II CCD area-detector'
_diffrn_measurement_method       'profile data from \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0183
_diffrn_reflns_av_sigmaI/netI    0.0133
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       7
_diffrn_reflns_limit_k_min       -7
_diffrn_reflns_limit_l_max       18
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            1160
_diffrn_reflns_theta_full        40.00
_diffrn_reflns_theta_max         40.00
_diffrn_reflns_theta_min         3.97
_exptl_absorpt_coefficient_mu    43.833
_exptl_absorpt_correction_T_max  0.2179
_exptl_absorpt_correction_T_min  0.1493
_exptl_absorpt_correction_type   analytical
_exptl_absorpt_process_details   'SADABS v2.03 (Bruker, 2003)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    8.000
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             350
_exptl_crystal_size_max          0.07
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         1.562
_refine_diff_density_min         -1.739
_refine_diff_density_rms         0.318
_refine_ls_extinction_coef       0.0094(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.181
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     12
_refine_ls_number_reflns         186
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.181
_refine_ls_R_factor_all          0.0197
_refine_ls_R_factor_gt           0.0179
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0191P)^2^+0.9329P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0405
_refine_ls_wR_factor_ref         0.0410
_reflns_number_gt                175
_reflns_number_total             186
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm501522v_si_003.cif
_cod_data_source_block
;
;
_cod_depositor_comments
'Adding full bibliography for 4001989--4001991.cif.'
_cod_original_sg_symbol_H-M      I4/mmm
_cod_database_code               4001991